1 Journal of Applied Electrochemistry 29: 703±717, Ó 1999 Kluwer Academic Publishers. Printed in the Netherlands. Time-dependent polarization behaviour of pipeline grade steel in low ionic strength environments S.L. CARSON and M.E. ORAZEM* Department of Chemical Engineering, University of Florida, Gainesville, FL , USA (*author for correspondence, Received 12 December 1997; accepted in revised form 18 August 1998 Key words: calcareous deposits, cathodic protection, polarization Abstract A bench-top experimental approach is described for estimation of the polarization behaviour of pipeline steel as a function of the time-dependent formation of scale and calcareous deposits in simulated soil leachates. A three-time constant process model provided a common set of parameters for a given soil environment and level of aeration. The parameters estimated could be applied to a broad range of current values and were independent of time, potential and applied current. The experimental approach, model and regression procedure are general and could be used to determine the physical parameters associated with the seasonal variations (wet±dry cycles) in the soils surrounding pipelines or with other factors that in uence general corrosion. The polarization model could provide a boundary condition for mathematical models for cathodic protection of pipelines or other buried structures. The separation of current contributions implicit in the model can be used to assess the reduction of corrosion current associated with speci c CP criteria. List of symbols a 0 a m b n E E comp;k E IR;k E meas;k E pred;k EFe E H 2 DE k F constant in the time-domain measurement model, Equation 17 (V) constant in the time-domain measurement model, Equation 17 (V) constant in the time-domain measurement model, Equation 17 (V) potential, Equation 10 (V) calculated IR compensated potential, Equation 3 (V) measured o -potential, Equation 1 (V) measured on-potential, Equation 3 (V) predicted on-potential, Equation 1 (V) reference potential for corrosion reaction, Equation 13 (V) reference potential for hydrogen evolution reaction, Equation 10 (V) Ohmic drop at time t k, Equation 2 (V) objective function, Equation 15, ma m 2 ffe exponential decay function, Equation 11 (dimensionless) f 1;Fe nal reaction current fraction, Equation 12 (dimensionless) f H2 exponential decay function, Equation 8 (dimensionless) f 1;H2 nal reaction current fraction, Equation 9 (dimensionless) f O2 exponential decay function, Equation 6 (dimensionless) f 1;O2 nal reaction current fraction, Equation 7 (dimensionless) I appl;k applied current, Equation 2 (ma) i Fe iron oxidation current density, Equation 5 (ma m 2 ) i Fe initial current density, Equation 11 (ma m 2 ) i H2 hydrogen evolution current density, Equation 5 (ma m 2 ) i H 2 initial current density, Equation 8 (ma m 2 ) ik applied current density at time t k, Equation 15 (ma m 2 ) ^ik model current density at time t k, Equation 15 (ma m 2 ) oxygen reduction current density, Equation 5 (ma m 2 ) mass transfer-limited oxygen reduction current, Equation 6 (ma m 2 ) i total net current density, Equation 5 (ma m 2 ) i O2 i O 2
2 704 R cell;k R cell;lm R cell;mean t k V meas V mod cell resistance at time t k, Equation 2 (X) time-varying cell resistance, Equation 4 (X) constant cell resistance, Equation 3 (X) time point, Equation 16 (s) measured potential, Equation 16 (V) model value of the potential, Equation 16 (V) Greek symbols b Fe Tafel slope for iron oxidation, Equation 13 (V (decade) 1 ) b H2 Tafel slope for hydrogen evolution, Equation 10 (V (decade) 1 ) e k U ref s Fe s H2 s m s n s O2 residual error, Equation 16 (V) reference electrode potential, Equation 17 (V) time constant for iron oxidation, Equation 12 (days) time constant for hydrogen evolution, Equation 9 (days) measurement model time constant, Equation 17 (days) measurement model time constant, Equation 17 (days) time constant for oxygen reduction, Equation 7 (days) 1. Introduction This work was motivated by the need to determine the electrochemical properties of steel as a function of time for two related applications. The rst application was to nd a method to establish suitable criteria for cathodic protection. Presently, several criteria are used to indicate that satisfactory levels of cathodic protection have been achieved [1±3]. In one criterion, cathodic protection is assumed to have been achieved if the applied current shifts the steel potential a set amount (e.g., 100 mv) from the depolarized corrosion potential. In another, an IR-corrected potential reading of ±850 mv (Cu/CuSO 4 ) is assumed to indicate that satisfactory protection has been achieved. It can be expected that the environment of the pipe will in uence the corrosion current seen at any given applied potential; thus, a method is needed to determine whether the corrosion current is reduced su ciently when such criteria are applied. The second application was to provide a method to establish parameters for polarization curves that can be used in mathematical models for cathodic protection which account for the electrochemistry at steel surfaces (e.g., [4±13]). At cathodic potentials, calcareous and rust scales can form due to localized alkalinity associated with oxygen reduction or hydrogen evolution at the steel surface . The similar values for the time constants associated with mass transfer transients and those associated with changes in scale thickness or resistance complicates measurement of polarization parameters for steel in soil and seawater environments . A dynamic potential or current scan must be conducted slowly enough to avoid artifacts associated with transient accumulation or depletion of ionic species in the di usion layer and fast enough that the changes in current and potential do not disrupt or alter the calcareous and scale deposits. In practice, there is no suitable scan rate that can be applied to obtain artifactfree potentiodynamic or galvanodynamic polarization curves . In this paper, a method is described which provides an estimate for time-dependent polarization curves. The experimental approach followed that of Nisancioglu et al. [4, 15] in which a polarization curve is constructed from a family of galvanostatic experiments conducted for a given environment. The mathematical formulation of the polarization curve represents an extension to that described by Nisancioglu et al. [4±6, 15], and model parameters were obtained by regression to the family of galvanostatic potential±time traces. Once the model parameters were estimated, e ective current±potential curves could be calculated for any desired time. The design of the model allowed the determination of the contributions of the individual reactions to the total current at any desired time and therefore could be used to establish the e ect of meeting a speci c CP criterion. The time-dependent polarization behaviour of steel can be obtained for di erent aqueous environments. The focus of the present work was on low ionic-strength, high-moisture content sand- lled environments which are intended to simulate real soil environments . 2. Background At potentials cathodic to the corrosion potential of steel, reduction of water and of dissolved oxygen causes the ph near the steel surface to be higher than that in the surrounding soil [14, 17]. The high cation concentration at the steel surface needed to satisfy electroneutrality facilitates precipitation reactions [14, 17]. Precipitation of calcium carbonate and magnesium carbonate can occur in the presence of carbonate or bicarbonate ions.
3 705 The source of carbonate ions in natural waters can be a mineral leachate or a product of dissolved carbon dioxide associated with aeration . Magnesium hydroxide, which can precipitate at ph values higher than 9.5, is also observed in calcareous lms [17, 18]. Calcareous deposits formed in sea water have been found to contain sodium, iron, silicon and strontium . In natural groundwaters, the cation content is a function of the mineral content of the surrounding soil . Calcareous deposits reduce corrosion rates by providing a barrier to mass transfer of oxygen or by inhibiting the hydrogen evolution reaction [4±6, 15]. In this paper, the corrosion reaction is treated as being inhibited by calcareous deposition. Deslouis et al.  report that the calcareous deposits formed under cathodic protection in waters containing both Ca 2 and Mg 2 consist of calcite and argonite crystals and has both a partial blocking and a porous behaviour. The formation of calcareous deposits reduces the amount of current required to achieve a given level of cathodic polarization and, therefore reduces the current requirements for cathodic protection . The e ects of calcareous deposition on the potential±current behaviour of a steel surface have been studied for synthetic and natural sea waters [4±6, 15], but a similar mechanistic study has not been done for the in uence of calcareous deposits in soil leachates which have a much lower ionic content. 3. Experimental method The experimental approach followed that of Nisancioglu et al. [4, 15] in which polarization parameters are constructed from a family of galvanostatic experiments conducted for a given environment. Application of constant current was chosen because, in potentiostatic experiments, both the current and the surface overpotential change in response to changes in the ohmic potential drop Cell design Cylindrical coupons, approximately three inches in length and one-half inch in diameter, were milled out of API5LX52 pipeline steel. The coupons were ultrasonically cleaned in ethanol and in distilled water before use, but other metallurgical pretreatment such as polishing or annealing was not used. Platinum served as the counter electrode to the 5LX52 steel. The cell (Figure 1) consisted of the API5LX52 cylindrical working electrode placed at the centre of a 5:41 cm (2.13 in) radius Nalgene jar with four 0:635 cm (0.25 in) strips of platinum (0:025 mm thick) placed 90 apart at a distance of 4:75 cm (1.87 in) from the centre of the cell . The symmetric placement of more than one counter electrode around a working electrode increased the uniformity of current distribution with respect to use of a single counter electrode . A calomel reference electrode was placed between two counter electrodes (45 from either anode) at a distance 4:1 cm (1.6 in) from the centre of the cell. The bottom circular surface of the steel electrode was masked by a thin epoxy (Hexcel Epolite 2410) disc. Both working and counter electrodes had a perpendicular contact with the bottom of the cell. This design provided a uniform distribution of current without completely encircling the working electrode with platinum. The current distribution for the working electrode surrounded by four anodes was calculated using the boundary element model described in  to be uniform to within better than 0.1% of the mean applied current density. Electrolyte replenishment was needed to avoid transients associated with changes in electrolyte composition. Electrolyte was dripped down a tube installed normal to the bottom of the cell, located approximately 0:635 cm (0.25 in) from the center of the cell between two anodes (45 from each) and 90 from the reference electrode. This design avoided formation of ground loops between cells. An outlet tube was placed on the side of the cell approximately 3 cm (1.2 in) from the bottom. The electrolyte level did not extend above the level of this outlet. Eight cells of this design were immersed in a temperature-controlled water bath maintained at a temperature of 20 2 C. Electrolyte was prepared in 50 L of deionized water. The oxygen content of the electrolyte was controlled by sparging either industrial grade Argon or air scrubbed of CO 2 by passing it through Ascarite II. The sparging process was begun 24 h prior to the addition of ionic species. The oxygen content after deaeration ranged from 1.5 to 3:5 ppm, and the oxygen content after aeration ranged from 7.5 to 8:5 ppm. Aeration or deaeration was maintained throughout the experiment. Aeration of electrolyte droplets by contact with air was minimized by maintaining a hydrated Argon atmosphere inside the tube. The hydrated gas produced from the reservoir bubbler was released into the atmosphere for the aerated electrolyte experiments and into the drip tubes for the deaerated electrolyte experiments. The electrolyte feed tube was split into eight lines and electrolyte was fed into each cell. The ow rate was monitored using glasstube Te on-bead owmeters. All experiments were performed in an inert solid matrix (silicate sand) to inhibit any convection in the cells.
4 706 Fig. 1. Design of experimental cell. Steel working electrode located in centre of cell is surrounded by a network of platinum counter electrodes. SCE between two platinum electrodes is for sensing. Electrolyte is constantly replenished by dripping feed into cell. Liquid level of cell is maintained by electrolyte dripping from outlet Data acquisition A Gamry Instruments PC3 potentiostat/galvanostat/ ZRA Board was installed in a personal computer and connected to a Gamry Instruments ECM8 electrochemical multiplexer. The multiplexer allowed eight cells to be simultaneously and independently controlled. The Gamry hardware was controlled using the Gamry CMS100 and CMS208 software packages. Hardware and code were developed to convert the ECM8 potentiostat into a galvanostat. The CMS208 galvanic corrosion routine was altered and used to apply a constant potential across a 1000 X resistor. A constant current was thereby applied between the working and counter electrode by connecting the working electrode to the resistor and connecting the counter and reference electrodes to the ECM8. A ltering procedure was used to reduce stochastic noise in the potential and current measurements. Twenty points were collected over 2.0 s. Current±time values and potential±time values were then t to a line using least squares regression. The value of the line at the last sample time was stored as the value for that sample. To reduce the e ect of switching multiplexer channels when a cell was sampled, the multiplexer was switched to the channel of a cell for one second prior to sampling. Determination of the ohmic drop in each cell during the experiment was required for analysis of the data. Continuous IR compensation by current interruption was found to be unreliable; thus, the current was interrupted periodically for a small number of measurements. The CMS208 galvanic corrosion code was modi ed such that the on-potential of the steel electrode was measured for 100 points after which ve o potentials were measured using a current interrupt technique. This cycle was repeated throughout the experiment Data conversion Current values were measured as the total current applied through the cell. Upon the completion of an experiment, each electrode was removed and the active surface height (exposed depth of the electrode in the
5 707 electrolyte) was measured, from which the active surface area was calculated. The cell resistance was calculated using the ohmic drop determined from the on-potential and o -potential measurements. A line was t to the ve points collected just before and the ve points collected just after the set of ve current interrupt measurements using a least squares algorithm. The resulting line was used to predict the values of potential measurement including ohmic drop, E pred;k, at the time, t k, of sampling of the currentinterrupt point. The di erence was calculated between the predicted potential including ohmic drop and the IR compensated measured potential, E IR;k : DE k ˆ E IR;k E pred;k 1 The di erence was then divided by the current applied, I appl;k, at that sampling time resulting in a value for the cell resistance R cell;k ˆ DE k I appl;k 2 IR compensation was obtained using either the mean value of R cell;k for the entire experiment, that is, E comp;k ˆ E meas;k I appl;k R cell;mean 3 or, for cases where the cell resistance was a function of time, using a cell resistance calculated for each set of ve current interrupt measurements P 5 kˆ1 R cell;lm ˆ R cell;k 5 4 The previous 100 potential measurements were corrected for ohmic drop using this mean value Electrolyte Two of the three electrolyte types employed in these experiments were selected to be consistent with previously analysed soil types . One soil was relatively rich in both Ca 2 and Mg 2 and is labelled here as electrolyte HCHM. The other soil was relatively rich in Ca 2 but not in Mg 2 and is labeled here as electrolyte HCLM. Electrolyte HCLM has a lower ionic strength than electrolyte HCHM. The concentrations of the ionic species in each electrolyte type are given in  and Table 1. The soil leachates were reproduced by dissolving appropriate amounts of reagent grade Ca(OH) 2, CaCl 2, K 2 SO 4, MgSO 4, Na 2 SO 4, and NaHCO 3 in 50 L of Table 1. Concentrations of electrolytes simulating soil types described by Han  Species HCLM electrolyte HCHM electrolyte /mol /ppm /mol /ppm Na K Ca Mg HCO mg dm mg dm 3 SO Cl Conductivity, 0.8 ± 1.9 ± /m X 1 cm 1 Ionic strength ± ± deionized water. As the leachate concentrations listed in reference  were not stoichiometrically balanced. Ca(OH) 2 and H 2 SO 4 were added in to reach the necessary concentrations of calcium and sulfate. The HCHM electrolyte required SO 2 4 concentrations far greater than could be added using the solid species; thus, excess H 2 SO 4 was added to reach the desired value. The solutions were titrated with NaOH and H 2 SO 4 solutions to reach the desired ph. Thus, the ionic strengths of the simulated leachates were greater than the reported values, but the concentrations of the species involved with deposition of calcareous deposits were consistent with reported values. Only the Na and SO 2) 4 concentrations were higher than reported by Han . 4. Polarization model The mathematical approach taken in the present work follows the model developed by Nisancioglu et al. [4±6, 15] to describe the time-dependent polarization relationship associated with formation of calcareous deposits with the exception that an additional relaxation process needed to be introduced in order to obtain a model of general applicability. Parameters were obtained by regressing the resulting model to all potential± time traces obtained for a given environment Physico-chemical model The total current to the surface i total ˆ i O2 i H2 i Fe 5 was assumed to consist of contributions from corrosion i Fe, oxygen reduction i O2, and hydrogen evolution i H2. The oxygen reduction reaction was assumed to be mass
6 708 transfer-limited, and the growth of calcareous deposits was assumed to reduce the value of the mass transferlimited current by a factor f O2 such that i O2 ˆ i O 2 f O2 6 where f O2 was assumed to have an exponential decay from an initial value of one to a long-time value f 1;O2 as f O2 f 1;O2 1 f 1;O2 ˆ exp t=s O2 7 The growth of calcareous deposits was assumed to reduce the value of the hydrogen evolution current by a factor f H2 such that i H2 ˆ i H 2 f H2 8 where f H2 f 1;H2 1 f 1;H2 ˆ exp t=s H2 9 The hydrogen reaction was assumed to be kinetically controlled, that is, i H 2 ˆ 10 E E H 2 b H2 10 As Equation 10 shows no dependence on mass transfer, the manner in which calcareous lms were assumed to reduce the rate of hydrogen evolution is di erent than that envisioned for oxygen reduction. The lm may act to poison the reaction or act as a barrier to the formed hydrogen gas molecules. In contrast to the model presented by Nisancioglu et al. [4±6, 15], the calcareous deposits were assumed to reduce the current associated with corrosion. Thus, i Fe ˆ i Fe f Fe where and 11 f Fe f 1;Fe 1 f 1;Fe ˆ exp t=s Fe 12 i Fe ˆ 10 E E Fe =b Fe 13 This extension of the model of Nisancioglu et al. [4±6, 15] was motivated by results of a time-dependent measurement model analysis of several potential traces which indicated that three exponential decay time constants were resolvable from the data (see Appendix); whereas, the model of Nisancioglu et al. [4±6, 15] included only two time±dependent processes. The current can be expressed in terms of all polarization parameters as i ˆ i O 2 f 1;O2 1 exp t=s O2 Š i O 2 exp t=s O2 10 E E H =b H2 2 f1;h2 1 exp t=s H2 Š 10 E E H =b H2 2 exp t=sh2 10 E E Fe =b Fe f 1;Fe 1 exp t=s Fe Š 10 E E Fe =b Fe exp t=s Fe 14 The calcareous deposits were assumed to in uence only the preexponential terms in Equations 8 and 11 through the factors f H2 and f Fe, respectively. The Tafel slope parameters and e ective equilibrium potentials (Equations 10 and 13) were therefore assumed to be independent of both potential and time Regression procedure In addition to the use of an extra time constant to account for growth of calcareous deposits, the present work is distinguished from the previous approach by the manner in which model parameters were obtained. Nisancioglu et al. [4±6, 15] employed a stepwise procedure for parameter estimation. The mass transferlimited oxygen reduction current was obtained either through extrapolation of potentiodynamic scans or through use of mass transfer correlations. The Tafel slopes were assumed to have values corresponding to bare steel. The time constant for hydrogen evolution was assumed to have an in nitely large value; thus the time dependence on hydrogen evolution was e ectively removed from the model. The reduced set of unknown parameters was obtained by regression. Nonin nite values for s O2, the time constant associated with the exponential decay of the oxygen reduction current, were only found for total currents which were greater than 0:5 i O 2. The resulting parameter space was therefore valid only for cathodic currents larger than 0:5 i O 2, and the model parameters such as s O2 were found to be functions of current density. Within the present work, Equation 14 was regressed to a data set for each electrolytic environment (consisting of data from up to eight individual cells). An unweighted nonlinear least-squares technique was employed where the objective function
7 709 F ˆ Xn kˆ1 2 i k ^i k 15 was minimized and where i k is the applied current density at time t k and i k is the value of the current given by Equation 14. The Levenberg±Marquardt method  was used to obtain the set of eleven parameters in the model which minimized the value of Equation Results and discussion The physico-chemical model was regressed to galvanostatic data. Time-dependent current±potential curves could be synthesized for the environments for which the model was employed. The estimated parameter sets for each environment demonstrated consistency with prior ndings. Fig. 3. Model values corresponding to three potential±time traces shown in Figure Regression The current values applied to each of eight cells were selected to encompass potentials both anodic and cathodic to the open-circuit condition. The three potential±time traces for the aerated HCHM electrolyte shown in Figure 2 represent an anodic, a cathodic, and the open circuit condition. The potential values have been corrected for ohmic drop. The mean resistance of each cell was X. The bimodal character of the potential traces was shown to be consistent with minor uctuations of the electrolyte level in the cell. The model values corresponding to the three traces shown in Figure 2 are presented in Figure 3. The residual error for the regression is given by e k ˆ V meas t k V mod t k 16 where V meas and V mod are the measured and model values, respectively, for potential at time t k. The residual errors for the regression are presented in Figure 4. Even for the most cathodic current, which has the least adequate t, the residual errors were very small. The residual errors were of the order of 10 mv for the anodic and cathodic curves and 2 mv for the open-circuit curve. Fig. 2. Three representative potential±time traces at three applied currents: anodic 0:808 A m 2 75:1 ma ft 2 ; cathodic 0:251 A m 2 23:3 ma ft 2 ; and zero net current. Fig. 4. Residual errors between model values in Figure 3 and measured potential±time traces in Figure 2.
8 710 The larger errors at short times may be associated in part with uncertainty concerning the start-up time and initial surface condition. Potential data collected at extremely cathodic currents was often not used in these regressions. In some cases, the data showed discontinuous behaviour that was associated with nucleation, growth, and detachment of hydrogen bubbles. Bubble formation can a ect the potential at the surface by blocking the electrode surface (decreasing current density), by blowing o calcareous lm (increasing current density), and by introducing hydrodynamics near the surface that are di erent than the hydrodynamics exhibited in the other cells under study. Use of a common set of parameters for each environment over the potential range studied requires that convection be independent of the applied current Synthesized polarization curves The model parameters obtained by regression are presented in Table 2 for the environments evaluated in this study. The con dence intervals reported for these parameters are those determined by the regression. The parameters can be used to reconstruct a family of current±potential curves predicted using the model for speci ed times. The resulting set of current-potential curves for the aerated HCHM electrolyte is presented in Figure 5 for 0, 2, 5, 10, 30 and 50 h, and 10 days. The corresponding set of curves for the deaerated HCHM electrolyte is presented in Figure 6. The solid curve in Figures 5 and 6 that shows the most negative open circuit potential is the predicted curve at 10 days. The other solid curve is the predicted initial curve. The re ned model and regression technique allowed the model to predict the potential-time behaviour over a wider range of currents than was possible using the previous result of Nisancioglu et al. [4±6, 15] The open circuit potential decreased with time and reached a steady state very rapidly, within two days, of approximately 710 mv vs SCE. The potential induced by a cathodic current decreased signi cantly over two days. A highly anodic current was predicted to produce an increasing anodic potential with time. This result was the least reliable in that only one anodic current value was used for the regression procedure. The need to account for three time-dependent processes (see Appendix) demonstrates the in uence of the corrosion reaction even at cathodic potentials. A common set of model parameters for each environment over the potential range studied could be successfully estimated only by including a time-dependent corrosion reaction in the model. Without the transient corrosion current, the time-dependent polarization curves would Fig. 5. Current±potential curves with reaction time as a parameter for the aerated HCHM electrolyte system. Curves do not change after two days. Key: ( ) 0 h, ( ) 2 h, ( ) 5 h, ( ) 10 h, ( ) 30 h, ( ) 50 h and ( ) 10 days. exhibit a static anodic current, which is inconsistent with collected anodic data Identi cation of current contributions The structure of the physical model allowed for direct deconvolution of the time±dependent current±potential behaviour of the individual contributing reactions. The Fig. 6. Current±potential curves with reaction time as a parameter for the deaerated HCHM electrolyte system. Curves do not change after 5 h. Key: as for Figure 5.
9 711 Table 2. Parameters of the physical model for the system described in Section 3 Parameter Aerated HCHM Deaerated HCHM Aerated HCLM Deaerated HCLM f 1;O s O2 /day i /A O2 cm f 1;H E /V vs SCE ) ) ) ) H2 b H2 /mv dec s H2 /day f 1;Fe EFe /V vs SCE b Fe /mv dec s Fe /day current±potential curves for the corrosion, oxygen reduction and hydrogen evolution reactions are plotted in Figure 7 for the initial electrode conditions, the condition at 2 h, and the condition at 10 days for the steel electrode in the aerated HCHM environment. The change in the rate of each contributing reaction over time to the total current±potential curves for the deaerated HCHM system is shown in Figure 8. The oxygen reduction currents and the corrosion currents decrease to their nal value in under two hours (for each reaction, the two hour and 10 day curves are superimposed). The hydrogen evolution current decreased more slowly than the other two currents. As an example of the reduction in current required to maintain a constant applied potential, the process model predicts that a current density of approximately 3:44 A m ma ft 2 would be required initially to maintain an applied potential of 800 mv vs SCE. Over 10 days, Figure 7 illustrates that the corrosion current falls by 15%, the oxygen reduction current decreases by 50%, and the hydrogen evolution current diminishes by over 90%. Figure 6 shows that the overall reduction in current requirement at 800 mv vs SCE is 70%. The reduction over ten days in the contributing currents was less signi cant for steel in calcium-poor and magnesium-poor environments. The generated time-dependent current±potential curves for API5LX52 pipeline steel in the aerated and deaerated HCLM environments are shown in Figures 9 and 10, respectively. The current±potential curves for Fig. 7. Individual current-potential curves for the three contributing reactions (corrosion, oxygen reduction and hydrogen evolution) with time as a parameter for the aerated HCHM electrolyte system. Oxygen reduction and corrosion contributions do not change after 2 h. Key: ( ) initial, ( ) 2 h and ( ) 10 days. Fig. 8. Individual current±potential curves for the three contributing reactions (corrosion, oxygen reduction and hydrogen evolution) with time as a parameter for the deaerated HCHM electrolyte system. Corrosion contribution does not change signi cantly over 10 days. Hydrogen evolution current changes more dramatically than oxygen reduction current. Key: as for Figure 7.
10 712 Fig. 9. Current±potential curves with reaction time as a parameter for the aerated HCLM electrolyte system. Curves do not change after two days. Key: ( ) 0 h, ( ) 2 h, ( ) 5 h, ( ) 10 h, ( ) 30 h, ( ) 50 h and ( ) 10 days. the corrosion, oxygen reduction, and hydrogen evolution reactions are plotted in Figure 11 (aerated HCLM) and Figure 12 (deaerated HCLM) for the initial electrode conditions, the condition at 2 h, and the condition at 10 days for the steel electrode in the aerated HCLM environment. The behaviour of the three reactions is similar for the HCHM and HCLM electrolyte systems. Fig. 11. Individual current±potential curves for the three contributing reactions (corrosion, oxygen reduction and hydrogen evolution) with time as a parameter for the aerated HCLM electrolyte system. Oxygen reduction and corrosion contributions do not change after 2 h. Key: ( ) initial, ( ) 2 h and ( ) 10 days. Under aeration, the oxygen reduction currents and the corrosion currents decrease to their nal value in under 2 h (for each reaction, the two hour and 10 day curves are superimposed). The hydrogen evolution current decreases more slowly than the other two currents. Under an argon atmosphere, the hydrogen evolution Fig. 10. Current±potential curves with reaction time as a parameter for the deaerated HCLM electrolyte system. Curves do not change after 10 h. Key: as for Figure 9. Fig. 12. Individual current±potential curves for the three contributing reactions (corrosion, oxygen reduction and hydrogen evolution) with time as a parameter for the deaerated HCLM electrolyte system. Corrosion contribution does not change signi cantly over 10 days. Hydrogen evolution current changes more dramatically than oxygen reduction current. Key: as for Figure 11.
11 713 reaction decays more rapidly and to a greater extent than the oxygen reduction reaction. The deconvolution of the model results suggests that the aeration level of the electrolyte is more important to the changes in reaction rates than is the concentration of calcareous ions. Comparison between the curves predicted for the aerated and deaerated HCLM electrolyte system (Figures 9 and 10) suggests that the potential drop at open circuit are nearly equal. However, the shape of the curves in the two cases is quite dissimilar. Predictions for the aerated case show de nite in ection points at very cathodic potentials which is consistent with the hydrogen evolution reaction becoming the dominant reaction in the system. The predicted curves for the deaerated case do not exhibit any such in ection point resulting from the lack of oxygen in the system. Thus, the model, in each case, behaves in a way which is consistent with the electrochemistry of the system Model parameters Although a larger sample of electrolyte compositions should be used to con rm the results obtained here, a Fig. 13. Model parameters of the corrosion current as a function of calcium concentration. Connected points are of the same aeration content electrolytes. (a) Steady state contributing current fraction; (b) time constant; (c) reference potential; (d) Tafel slope. Key: ( h ) aerated and ( e ) deaerated.
12 714 preliminary interpretation of the in uence of aeration and ionic content on the regressed parameter values can be made Corrosion The values of the parameters associated with the corrosion reaction are plotted in Figure 13 against the calcium content of the various electrolytes tested. The dashed lines represent the con dence interval obtained by regression. The steady state contributing current fraction parameter f 1;Fe was found to be independent of dissolved oxygen level or calcium content. This nding is consistent with the assumption made by Nisancioglu, et al. [4±6, 15] that the cathodic reactions do not a ect the rate of corrosion of steel. The time constant s Fe associated with the corrosion reaction was a ected by dissolved oxygen content, suggesting that the corrosion reaction reaches its steady rate more slowly in deaerated electrolytes than in aerated environments. The two kinetic parameters, EFe and b Fe, were independent of dissolved oxygen content or calcium concentration. The independence of the two parameters with respect to aeration and calcium content is consistent with the assumption that EFe and b Fe are independent of time. Fig. 14. Model parameters of oxygen reduction current as a function of calcium concentration. Connected points are of the same aeration content electrolytes. (a) Steady state contributing current fraction; (b) time constant; (c) mass transfer-limited oxygen reduction current. Key: ( h ) aerated and ( e ) deaerated.
13 Oxygen reduction Many of the parameters associated with the reduction of oxygen were dependent on aeration level (Figure 14). More data are needed to determine the dependence of f 1;O2 on the dissolved oxygen content or on calcium concentration. The dependence of f 1;O2 on electrolyte composition is an important issue. If the parameter is constant for all dissolved oxygen and calcium concentrations, the same level of protection should eventually be obtained for any calcium content or aeration level. The time constants associated with the reduction of oxygen, s O2, and the mass transfer-limited oxygen reduction current, i O 2, were clearly dependent upon dissolved oxygen content. The time constant was larger for the reaction in deaerated electrolytes; therefore, the barrier to the transport of oxygen was formed more rapidly in deaerated environments than in aerated electrolytes. The mass transfer-limited oxygen reduction current was generally larger in aerated electrolytes Hydrogen evolution The parameters associated with the hydrogen evolution reaction are presented in Figure 15. The steady state contributing current fraction f 1H2 showed no distinct Fig. 15. Model parameters of the hydrogen evolution current as a function of calcium concentration. Connected points are of the same aeration content electrolytes. (a) Steady state contributing current fraction; (b) time constant; (c) reference potential; (d) Tafel slope. Key: ( h ) aerated and ( e ) deaerated.
14 716 trending with aeration level or calcium concentration. The time constant for the reaction s H2 was strongly dependent on dissolved oxygen content. The hydrogen evolution reaction achieved a steady state more rapidly in aerated environments than in deaerated environments. The two kinetic parameters, EH 2 and b H2, were independent of the dissolved oxygen and calcium concentrations. The small time constants for oxygen reduction and hydrogen evolution obtained in the present work are consistent with recent results obtained for synthetic and natural seawater [18, 20]. The results of these regressions are consistent with the values of 0:1 ma cm 2 reported by Han  for the mass transfer-limited oxygen reduction currents in saturated HCLM and HCHM environments. The mass transfer-limited oxygen reduction current and the hydrogen evolution potential driving force would be of smaller magnitudes in drier soils . Literature values for the Tafel slopes and equilibrium potentials for the hydrogen evolution and corrosion reactions are probably inappropriate for surfaces covered by calcareous lms. The values obtained in this work for hydrogen evolution, for example, are on the order of 400 mv (decade) 1 as opposed to the value of 174 mv (decade) 1 assumed by Nisancioglu et al. [4±6, 15] Perhaps the most compelling argument in favour of the method used in this work is that the resulting parameters were found to be constants for a given environment. A common set of parameter values was found to apply for all measurements made at a given electrolyte composition and oxygen content. The success of the model is evident in that a t to within less than 20 mv was obtained with parameters that were not functions of time or potential Application to CP criteria The large Tafel slopes obtained in this work for the corrosion reaction imply that large shifts in potential are needed to reduce the corrosion current to a smaller value. For example, the value of Tafel slope reported in Table 2 means that a 924 mv shift is required to reduce the corrosion current by an order of magnitude. The magnitude of the Tafel slope, which is much larger than the 60 mv value expected for bare steel, can be attributed in part to the potential dependence of the calcareous deposits. The polarization requirements described here for a saturated soil matrix are much more severe than those reported for damp soils . The experimental technique and associated regression procedure could be employed for soils of controlled moisture content to obtain values more representative of eld applications. 6. Conclusions The experimental system described provided bench-top measurements of the current±potential±time response of pipeline steel to formation of deposits in electrolytes designed to simulate soil leachate compositions. The system was designed to provide uniform current and potential distributions over the electrodes; thus the analysis did not require correction for nonuniform reaction kinetics. All experiments were performed in an inert solid matrix (silicate sand). Replenishment of electrolyte was required to avoid pitting on the steel surface. The time constants for the in uence of the growth of calcareous deposits and corrosion products in uence the overall current response at cathodic potentials near the corrosion potential. The three-time constant process model used to describe the results provided a common set of parameters for a given soil environment and level of aeration. The parameters estimated were valid for all applied current values and were independent of time, potential and applied current. The experimental approach and regression procedure model used are general and could be used to determine the physical parameters associated with the seasonal variations (wet±dry cycles) in the soils surrounding pipelines or with other factors that in uence general corrosion. The polarization model provides critical information that could be used as a boundary condition in mathematical models for cathodic protection of pipelines or other buried structures. The separation of current contributions implicit in the model can be used to assess the reduction of corrosion current associated with speci c CP criteria. Acknowledgements This work was supported by PRC International via Contract RPTG/PR: 101±9221. A full report of  is available from the American Gas Association. The authors thank the Corrosion Supervisory Committee of PRC International for their oversight and suggestions. Appendix: Time-domain measurement model The frequency domain measurement model approach developed for spectroscopy measurements [24±31] was extended to provide a time-domain measurement model to extract the number of independent time-dependent processes represented in a potential±time trace. The
15 717 model accounted for processes leading to exponentially decaying increases or decreases in potential, that is, V U ref ˆ a 0 Xj Xk nˆ1 mˆ1 a m exp t=s m b n 1 exp t=s n 17 where a 0 P k nˆ1 b n represents the potential obtained as time approaches in nity. The model was regressed to individual potential±time traces using the Marquardt± Levenberg method . The requirement that the con dence interval for parameter estimates not exceed their 95.4% con dence interval was used to identify the maximum number of exponential lineshapes. Data taken from preliminary experiments in which the electrolyte was not replenished revealed an exponential decay followed by an exponential increase in potential. Visual inspection of the coupons after the experiment revealed corrosion by pitting. Once fresh electrolyte was fed continuously, pitting was no longer observed, and a time increasing function could no longer be regressed to the measured potential±time traces. With the exception of the most anodic and cathodic currents, three exponential decay lineshapes could be identi ed by the regression procedure. At very anodic currents, the hydrogen evolution reaction is expected to provide a negligible contribution to the total current. Likewise, the corrosion reaction current is expected to be insigni cant at very cathodic currents. The time decay processes were taken to be associated with the e ect that the formation of lms would have on the three contributing reactions. No lineshape associated with an increase in potential could be resolved from the data after the system was modi ed to refresh the electrolyte. References 1. A.W. Peabody, `Control of Pipeline Corrosion', NACE Publications, Houston, TX (1967). 2. J. Morgan, `Cathodic protection', 2nd edn (NACE Publications, Houston, TX 1993). 3. R.U. Lee and J.R. Ambrose, Corrosion 44 (1988) 887± K. Nisancioglu, Corrosion 43 (1987) 100± K. Nisancioglu, P.O. Gartland., T. Dahl and E. Sander, Corrosion 43 (1987) 710± K. Nisancioglu and P.O. Gartland, `Current Distribution With Dynamic Boundary Conditions', I. Chem. symposium Series No. 112: Conference on Electrochemical Engineering, Loughborough University of Technology, Loughborough UK (April, 1989). 7. S.N.R. Yan, Pakalapati, T.V. Nguyen, R.E. White and R.B. Gri n, J. Electrochem. Soc. 139 (1992) 1932±6. 8. K.J. Kennelley, L. Bone and M.E. Orazem, 49 (3) (1993) 199± S.N.R. Yan, Pakalapati, T.V. Nguyen, R.E. White and R.B. Gri n, J. Electrochem. Soc. 139 (1992) 1932± M.E. Orazem, L. Bone and K.J. Kennelley, Corrosion 49 (1993), 211± R.M. Degerstedt, K.J. Kennelley, M.E. Orazem and J.M. Esteban, Mater. Perform. 35 (1996) 16± M.E. Orazem, J.M. Esteban, K.J. Kennelley and R.M. Degerstedt, Corrosion 53 (1997) 264± M.E. Orazem, J.M. Esteban, K.J. Kennelley and R.M. Degerstedt, Corrosion 53 (1997) in press. 14. W.H. Hartt, C.H. Culberson and S.W. Smith, Corrosion 40 (1984) 609± K. Nisancioglu, in `Modern Aspects of Electrochemistry' Vol. 23 (edited by R. White, J. O'M Bockris and B. E. Conway, (Plenum Press, New York, 1992), p M.K. Han, `E ects of Seasonal Variations on Requirements to Prevent Corrosion in Soils', Final Report PR to the Corrosion Supervisory Committee of the American Gas Association (Dec. 1988). 17. J. J. Morgan and W. Stumm, `Aquatic Chemistry: An Introduction Emphasizing Chemical Equilibria in Natural Waters' (John Wiley & Sons, New York, 1981). 18. O. Gil, S. Touzain, C. Deslouis, B. Tribollet, C. Compere and D. Feisty, `In situ characterization of calcareous layers formed in synthetic sea water', presented at the 3rd International Symposium on Electrochemical Impedance Spectroscopy, 7±12 May (1995), Nieuwpoort, Belgium. 19. J.S. Luo, R.U. Lee, T.Y. Chen, W.H. Hartt and S.W. Smith, Corrosion 47 (3) (1991) 189± C. Deslouis, A. Doncescu, D. Feisty, O. Gil, V. Maillot, S. Touzain and B. Tribollet, `Kinetics and characterization of calcareous deposits under cathodic protection in natural seawater', presented at the 6th International Symposium on Electrochemical Methods in Corrosion Research, 25±29 Aug. (1997), Trento, Italy. 21. M.E. Orazem and S.L. Carson, `Time-Dependent Polarization behaviour as a Function of Soil Type', Catalogue L51735, PRC International at the American Gas Association, Arlington, VA (1995). 22. J. Newman, J. Electrochem. Soc. 138 (1991) 3554± W. H. Press, B. P. Flannery, S. A. Teukolsky and W. T. Vetterling, `Numerical Recipes: The Art of Scienti c Computing (FORTRAN Version)' (Cambridge University Press, 1989). 24. P. Agarwal, M. E. Orazem and LH. GarcõÂ a-rubio, J. Electrochem. Soc. 139 (1992) 1917± P. Agarwal, O. C. Moghissi, M. E. Orazem and L.H. GarcõÂ a- Rubio, Corrosion, 49 (1993) 278± M. Orazem, P. Agarwal, A.N. Jansen, P.T. Wojcik and L.H. GarcõÂ a-rubio, Electrochem. Acta 38 (1993) 1903± P. Agarwal, Oscar D. Crisalle, M. E. Orazem and L.H. GarrcõÂ a- Rubio, J. Electrochem. Soc. 142 (1995) 4149± P. Agarwal, M.E. Orazem and L.H. GarcõÂ a-rubio, J. Electrochem. Soc. 142 (1995) 4159± M.E. Orazem, P. Agarwal and L.H. GarcõÂ a-rubio, Mater. Sci. Forum 192±194 (1995) 563± M.E. Orazem, P. Agarwal, C. Deslouis and B. Tribollet, J. Electrochem. Soc. 143 (1996) 948± M.E. Orazem, T. El Mousta d, C. Deslouis and B. Tribollet, J. Electrochem. Soc. 143 (1996) 3880±90.
16 COPYRIGHT INFORMATION TITLE: Time-dependent polarization behaviour of pipeline grade steel in low ionic strength SOURCE: J Appl Electrochemnlectronl 29 no62217/12 Je The magazine publisher is the copyright holder of this article and it is reproduced with permission. Further reproduction of this article in violation of the copyright is prohibited. To contact the publisher:
Measurements of corrosion rate on Carbon-steel using Electrochemical (potentiodynamic Polarization, EIS etc.) technique. Corrosion Rate Measurement on C-Steel Abdullah Al Ashraf 1. Introduction: The degradation
JOURNAL OF APPLIED ELECTROCHEMISTRY 28 (1998) 811±817 Electrochemical reduction of nitrates and nitrites in alkaline media in the presence of hexavalent chromium H. A. DUARTE, K. JHA, J. W. WEIDNER* Department
Lecture - 40 Laboratory Experiments in Corrosion Engineering II Keywords: Polarization Experiments, Pitting Potentials, Microbial Corrosion. A. Electrochemical tests in a given environment Polarization
Data Sheet CORROSION CONTROL Corrosion control is the application of engineering principles and procedures to minimise corrosion to an acceptable level by the most economical method. It is rarely practical
Assignments 1. Prepare Galvanic series for metals and alloys in flowing sea water. Compare this with the series available for stagnant sea water. 2. Construct the Eh ph diagram for the Zn H 2 O O 2 system
5th International Conference on Durability of Concrete Structures Jun 30 Jul 1, 2016 Shenzhen University, Shenzhen, Guangdong Province, P.R.China Threshold Chloride Concentration of Stainless Steels in
Application Note CORR-4 Subject: Electrochemistry and Corrosion: Overview and Techniques INTRODUCTION During the late 70 s and early 80 s, corrosion specialists began to discover that electrochemical (ECHEM)
SHAW AND ASSOCIATES CONSULTING Galvanic corrosion evaluation of 6061 aluminum coupled to CVD coated stainless steel Elizabeth Sikora and Barbara Shaw 6/9/2016 Evaluation of galvanic corrosion of aluminum
1 Iron is extracted from the ore hematite in the Blast Furnace. waste gases firebrick lining raw materials: coke, C iron ore, Fe 2 O 3 limestone, CaCO 3 CO forms air slag molten iron CO 2 forms (a) The
7th Pipeline Technology Conference 2012 Effect of Precorrosion and Temperature on the Formation Rate of Iron Carbonate Film Winia Farida a,b, Tor Hemmingsen b, Tonje Berntsen b,c, Patrick Rabindran a a
Boiler Water Problems and Its Causes Water is the essential medium for steam generation. Conditioning it properly can increase the efficiency of boiler and as well as extend the boiler s life. Treating
CORROSION BEHAVIOR OF TITANIUM METAL IN PRESENCE OF INHIBITED SULFURIC ACID AT 50 o C 1 Ismaeel N. Andijani, Shahreer Ahmad and Anees U. Malik Research & Development Center Saline Water Conversion Corporation
ACCELERATED CORROSION TESTING OF GALVANIC COUPLES James F. Dante, Josh Averett, Fritz Friedersdorf, and Christy Vestal Luna Innovations 706 Forest St. Suite A Charlottesville, VA 22903 email@example.com
ABSTRACT IN SITU MONITORING OF REINFORCEMENT CORROSION BY MEANS OF ELECTROCHEMICAL METHODS Oskar Klinghoffer, M.Sc. FORCE Institute, Park Allé 345, DK-2605 Brøndby, Denmark The well-known and usually adapted
Circular No. 61 1957 STATE OF ILLINOIS WILLIAM G. STRATTON, Governor by R. V. SKOLD AND T. E. LARSON Issued by DEPARTMENT OF REGISTRATION AND EDUCATION VERA M. BINKS, Director STATE WATER SURVEY DIVISION
Paper No. 3880 Effect of Chloride on Localized Corrosion Initiation of Carbon Steel in a CO 2 Aqueous Environment Xin Gao, Bruce Brown, Srdjan Nesic Institute for Corrosion and Multiphase Technology Ohio
Distribution Review Corrosion Control Corrosion Control Training Objectives To gain an understanding of: Corrosion control vocabulary The factors affecting corrosion Methods used to control corrosion Alkalinity
ONLINE MONITORING OF CORROSION UNDER CATHODIC PROTECTION CONDITIONS UTILIZING COUPLED MULTIELECTRODE SENSORS Xiaodong Sun Corr Instruments, LLC San Antonio TX, USA ABSTRACT Real-time corrosion monitoring
Paper No. CORROSION 200 0623 MODELING OF CO 2 CORROSION OF MILD STEEL AT HIGH PRESSURES OF CO 2 AND IN THE PRESENCE OF ACETIC ACID Keith George, Shihuai Wang, Srdjan Nesic and Kees de Waard Institute for
50 Corrosion and inhibition Behaviour of Aluminium in Alkaline Medium and Sodium Silicate. Manish Gupta 1 Jyotsna Mishra* 2 and K.S. Pitre 3 1, 2 Department of Engineering Chemistry, SCOPE College of Engineering,
Int. J. Electrochem. Sci., 2 (2007) 563-571 www.electrochemsci.org Corrosion and inhibition of Cu-Zn alloys in NaCl solution by using permanganate and phosphate anions S. A. M. Refaey 1, *, A. M. Abd El
Corrosion of platinum (Pt) in HCl Now if we place a piece of Pt in HCl, what will happen? Pt does not corrode does not take part in the electrochemical reaction Pt is a noble metal Pt acts as a reference
Studies on Alloys and Composites that Undergo Anomalous Codeposition Electrochemical of of South Columbia, SC908 09, 1998 Electrochemical Systems Studied FeNi alloys and FeNiSiO composites Electrodeposition
1 Two of the main uses of zinc are for galvanising and for making alloys. One of the main ores of zinc is zinc blende, ZnS. There are two stages in the extraction of zinc from this ore. (a) Stage 1 Zinc
196 Int. J. Microstructure and Materials Properties, Vol. 4, No. 2, 2009 The influence of Mg 17 Al 12 phase volume fraction on the corrosion behaviour of AZ91 magnesium alloy Andrzej Kiełbus* and Grzegorz
The Effect of Cl - and Acetic Acid on Localized CO 2 Corrosion in Wet Gas Flow Yuhua Sun, Keith George, and Srdjan Nesic NSF I/UCRC, Corrosion in Multiphase Systems Center Institute for Corrosion and Multiphase
IRON CARBONATE SCALE GROWTH AND THE EFFECT OF INHIBITION IN CO 2 CORROSION OF MILD STEEL Kunal Chokshi, Wei Sun, Srdjan Nesic Institute for Corrosion and Multiphase Technology, Ohio University 342 West
2017 Award Nomination Title of Innovation: Ultrasound Cathodic Protection Test Station Nominee(s) Eugene (Gene) B. Silverman PhD, Berkeley Springs Instruments LLC Category: Cathodic Protection Coatings
Outline Corrosion - Introduction Corrosion of Metals - e.g. Rusting of iron in water Electrochemical Cell Electrode Potential in Electrochemical Cell Standard Electromotive Force Example Relative Corrosion
What s Next Establishing Reassessment Intervals NACE ECDA Seminar Houston January 26- January 28 2009 Kevin C. Garrity, P.E. DNV Topics Covered Focus is ECDA - Reassessment Methodology, - Corrosion Growth
Electrochemistry Written Response January 1999 7. Balance the following redox reaction in acidic solution: RuO 4 + P Ru(OH) 2 2+ + H 3 PO 3 (acid) (3 marks) 8. A technician tests the concentration of methanol,
Propagation of Localised Corrosion: FEM Approach M. Stroe *,1, R. Oltra 1, B. Vuillemin 1, G. Girardin 2 1. Institut Carnot de Bourgogne (ICB), 2. AREVA NP *ICB, UMR 5209 CNRS-Université de Bourgogne,9
1 The reactivity series lists metals in order of reactivity. (a) To find out which is the more reactive metal, zinc or tin, the following experiment could be carried out. piece of zinc shiny surface tin(ii)
Materials Transactions, Vol. 51, No. 6 (21) pp. 119 to 1113 #21 The Japan Institute of Metals Effect of Anodizing Potential on the Surface Morphology and Corrosion Property of AZ31 Magnesium Alloy S. A.
Corrosion Science 42 (2000) 979±990 EIS studies of a corrosion inhibitor behavior under multiphase ow conditions Y. Chen*, T. Hong, M. Gopal, W.P. Jepson NSF I/UCRC, Corrosion in Multiphase Systems Center,
Electronic Supplementary Material (ESI) for ChemComm. This journal is The Royal Society of Chemistry 2014 Three-dimensional NiFe Layered Double Hydroxide Film for Highefficiency Oxygen Evolution Reaction
JOURNAL OF APPLIED ELECTROCHEMISTRY 28 (1998) 1389±1397 Material aspects of the liquid feed direct methanol fuel cell K. SCOTT, W. M. TAAMA, P. ARGYROPOULOS Chemical and Process Engineering Department,
REMOVAL OF HARDNESS BY PRECIPITATION Hardness divalent cations If hardness is too high Ca 2+ + Mg 2+ + Fe 2+ + Mn 2+ + Sr 2+... precipitation of soap, scaling on pipes, boilers, cooling towers, heat exchangers.
PIPELINE COATING FAILURE - NOT ALWAYS WHAT YOU THINK 1T IS Dennis Neal Harding & Neal, Inc. 10 Wild Oak Circle Houston, TX 77055 4724 ABSTRACT Corrosion coating failure has traditionally been defined by
Oxidation and Reduction An oxidation reaction is one in which oxygen is added to a substance. Example: Methane is oxidised when it burns in air. Oxygen is added to the carbon in methane, forming carbon
ELECTROCHEMICAL SYNTHESIS OF POLYPYRROLE (PPy) and PPy METAL COMPOSITES ON COPPER and INVESTIGATION OF THEIR ANTICORROSIVE PROPERTIES Sibel Zor, Hatice Özkazanç Kocaeli University, Department of Chemistry,
IOP Conference Series: Earth and Environmental Science PAPER OPEN ACCESS Corrosion and Protection of Metal in the Seawater Desalination To cite this article: Xiangyu Hou et al 018 IOP Conf. Ser.: Earth
Buried Pipe Corrosion in the Power Plant Environment Assessment and Mitigation in Nuclear Power Plants IAEA Technical Meeting on Buried Pipe October 15, 2014 Kurt M. Lawson Mears Group, Inc. Topics Background
Period 3 Elements 6 2 Sodium, aluminium and silicon are solid elements with a silver colour. These elements react with oxygen to form oxides with high melting points. Aluminium is a reactive metal, but
A STUDY OF PROTECTIVE IRON CARBONATE SCALE FORMATION IN CO CORROSION Wei Sun, Kunal Chokshi, Srdjan Nesic, and Daniel A. Gulino Institute for Corrosion and Multiphase Technology 4 West State Street Ohio
Stability of Surface Films Formed on Mg by Exposure Aqueous Solutions By: Mehdi Taheri Supervisor: Dr. Joseph Kish Walter W. Smeltzer Corrosion Lab McMaster University 1 2 nd MSE 702 Graduate Seminar Sept
APPLICATIONS OF ELECTROCHEMISTRY SPONTANEOUS REDOX REACTIONS APPLICATIONS OF ELECTROCHEMICAL CELLS BATTERIES A galvanic cell, or series of combined galvanic cells, that can be used as a source of direct
Dynamic Stray Current Interference Testing And Mitigation Design For A 90-Inch Water Main Authors: Rogelio de las Casas, Ron Turner, Kristi Roe; EN Engineering This paper discusses two sections of pipeline
CATHODIC PROTECTION Cathodic protection is a proven corrosion control method for protection of underground and undersea metallic structures, such as oil and gas pipelines, cables, utility lines and structural
ONLINE MONITORING OF UNDERCOATING CORROSIONS UTILIZING COUPLED MULTIELECTRODE SENSORS Xiaodong Sun Corr Instruments, LLC San Antonio TX, USA ABSTRACT Online monitoring of carbon steel corrosion under different
Int. J. Electrochem. Sci., 10 (2015) 1434-1446 International Journal of ELECTROCHEMICAL SCIENCE www.electrochemsci.org Cathodic Reaction Mechanism of 3Cr Low Alloy Steel Corroded in CO 2 -Saturated High
Simulation of Electrochemical Processes 59 Galvanic corrosion modeling in flowing systems D. A. Shifler 102 Potomac Street, Boonsboro, MD 21713-1211, USA Abstract Contact between dissimilar alloys will
Ductile Iron Piles Corrosion Resistance Ductile Iron Piles are often a preferred, cost-effective foundation support solution for a variety of projects particularly in urban settings. Similar to other types
Characteristics and efficiency of PEM fuel cell TEP Related Topics Electrolysis, electrode polarisation, decomposition voltage, galvanic elements, Faraday s law. Principle In a PEM electrolyser, the electrolyte
Evaluation of Zn-rich Primers and Rust Converters for Corrosion Protection of Steel Leonardo Caseres Southwest Research Institute Report Documentation Page Form Approved OMB No. 0704-0188 Public reporting
Lecture 20 Passivity Definitions and Influencing Parameters Keywords: Definition of Passivity, Flade Potential, Anodic Polarization, Critical Anodic Current Density. In the Eh ph diagrams, resistance to
Trace Elements in Carbonates A Short Course VU March, 2009 Peter Swart University of Miami Trace Elements and Minor Elements Minor Elements (Usually concentrations over 1000 ppm) Strontium Aragonite-7000
Indian Journal of Chemical Technology Vol. 15, March 2008, pp. 174-179 Corrosion characteristics of mild steel in aqueous solution of formic acid containing some acetic acid S K Singh, Ashim K Mukherjee*
2347 A publication of CHEMICAL ENGINEERING TRANSACTIONS VOL. 43, 2015 Chief Editors: Sauro Pierucci, Jiří J. Klemeš Copyright 2015, AIDIC Servizi S.r.l., ISBN 978-88-95608-34-1; ISSN 2283-9216 The Italian
A CORROSION MANAGEMENT AND APPLICATIONS ENGINEERING MAGAZINE FROM OUTOKUMPU Corrosion Properties of Enhanced Duplex Steel UNS S3234 2/215 2/215 2 Corrosion Properties of Enhanced Duplex Steel UNS S3234
Introduction to Cathodic Protection Course No: T02-004 Credit: 2 PDH J. Paul Guyer, P.E., R.A., Fellow ASCE, Fellow AEI Continuing Education and Development, Inc. 9 Greyridge Farm Court Stony Point, NY
ORIENTAL JOURNAL OF CHEMISTRY An International Open Free Access, Peer Reviewed Research Journal www.orientjchem.org ISSN: 0970-020 X CODEN: OJCHEG 2016, Vol. 32, No. (6): Pg. 2929-2937 Thermodynamics and
ISSN: 2321-4902 Volume 1 Issue 1 Online Available at www.chemijournal.com International Journal of Chemical Studies Calculation of Diffusion Coefficients and Layer Thickness for Oxidation the Ferrocene
Paper No. 11072 2011 Effect of FeCO Supersaturation and Carbide Exposure on the CO 2 Corrosion Rate of Carbon Steel Tonje Berntsen Statoil ASA P.O. Box 08 N-5501 Haugesund Norway Marion Seiersten Institute
PROF. DR. M.M. B. EL SABBAH AL-AZHAR UNIVERSITY FACULTY OF SCIENCE CHEMISTRY DEPARTMENT 2016 PRINCIPLES OF CORROSION ELECTROCHEMICAL AND THERMODYNAMIC PRINCIPLES OF CORROSION Content 1. Definition of corrosion.
Reviewers' comments: Reviewer #1 (Remarks to the Author): In this paper, Hersbach et al. reported an impressive study of the anisotropic etching of Pt electrodes at the onset of cathodic corrosion. This
Volume 13 September 007 SACRIFICIAL ANODE CATHODIC PROTECTION OF LOW CARBON STEEL IN SEA WATER Dr. Aprael S. Yaro Dr. Khalid W. Hameed University of Baghdad / College of Engineering ABSTRACT Cathodic protection
Introduction Jeremy Hailey, P.E. Engineer with 16 years experience Started NW 10 years ago Focus on corrosion control system designs, troubleshooting, and some installation work Conduct training seminars
Electrochemistry Communications 3 2001) 299±305 www.elsevier.nl/locate/elecom The voltage±time behaviour for porous anodizing of aluminium in a uoride-containing oxalic acid electrolyte A. Mozalev a, *,
Related topics Electrolysis, electrode polarisation, decomposition voltage, galvanic elements, Faraday s law. Principle and task In a PEM electrolyser, the electrolyte consists of a protonconducting membrane
Preface... xi Chapter 1. Metallurgical Thermochemistry... 1 1.1. Introduction... 1 1.2. Quantities characterizing the state of a system and its evolution... 3 1.2.1. The types of operations... 3 1.2.2.
International Journal of Basic & Applied Sciences IJBAS-IJENS Vol: 11 No: 06 75 Corrosion Behavior of Mild Steel in Seawater from Two Different Sites of Kuala Terengganu Coastal Area W.B. Wan Nik 1*, F.
ELECTROCHEMICAL REDUCTION OF TITANIUM DIOXIDE THIN FILM IN LiCl-KCl-CaCl 2 EUTECTIC MELT Yasushi Katayama Department of Applied Chemistry, Faculty of Science and Technology, Keio University 3-14-1, Hiyoshi,
NCERT solutions for Metals and Non Metals 1 Question 1 Give an example of a metal which (i) is a liquid at room temperature. (ii) can be easily cut with a knife. (iii) is the best conductor of heat. (iv)
Portugaliae Electrochimica Acta 22 (2004) 295-304 PORTUGALIAE ELECTROCHIMICA ACTA Semiconductor Electrochemistry and Localised Corrosion C.M. Rangel, * M. da Cunha Belo a,b Instituto Nacional de Engenharia
A STUDY OF CAUSTIC CORROSION OF CARBON STEEL WASTE TANKS C. F. Jenkins Westinghouse Savannah River Company Aiken, South Carolina, USA, 29808 ABSTRACT Solution chemistry of wastes from US atomic weapons
ELECTROCHEMICAL IMPEDANCE SPECTROSCOPY ON THERMAL AGEING EVALUATION OF EPOXY COATING CONTAINING ZINC RICH PRIMER Zalilah Sharer 1, John Sykes 2 1 UTM-MPRC, Institute for Oil and Gas, Universiti Teknologi
FINAL REPORT: LARGE SCALE ACCELERATED CUI TEST OF E-2000 AND E-1100EG Prepared for: Elisha Technologies Company L.L.C. P.O. Box 280 Moberly, Missouri 65270 Prepared by: Dr. Russell D. Kane InterCorr International,
Water Technologies & Solutions capability profile Solus* AP - advanced boiler all-polymer internal treatment technology a discussion in question and answer format 1. what is Solus AP boiler treatment technology?
DECOMPOSITION OF HYDRAZINE IN PRESERVED BOILERS 1 P.C.Mayan Kutty and T.S.Thankachan, Research & Development Center, Al Jubail Abdullah Al Ajlan and Ghazzai Al Mutairi, Laboratory Dept., SWCC Al-Jubail
International Journal of ChemTech Research CODEN (USA): IJCRGG, ISSN: 0974-4290, ISSN(Online):2455-9555 Vol.10 No.6, pp 617-621, 2017 Effect of Heat Treatment on the Behaviour of GTM- SU- Superalloy in
INSTITUTE OF INTEGRATED ELECTRICAL ENGINEERS OF THE PHILIPPINES, INC. () www.iiee-ercsa.org First IIEE Accredited Foreign Chapter (Charter No. 62) Most Outstanding Chapter Overseas for the year 1998, 1999,
Water Technologies & Solutions technical bulletin Steamate* technology superior protection against condensate system corrosion problems in steam distribution systems The steam distribution system can be
Lecture 18 Design Aspects of Cathodic Protection Keywords: Cathodic Protection Design, Choice of Protection, Engineering Aspects. Advantages and uses of cathodic protection: Compared to alternative protection
SCA2017-061 1/8 INVESTIGATION OF CO- AND COUNTER CURRENT FLOW BEHAVIOR IN CARBONATE ROCK CORES Pouyan Ahmadi 1, Masoud Riazi 1, Mohammad Reza Malayeri 1 1 EOR Research Center, School of Chemical and Petroleum
Numerical simulation of the cathodic protection of pipeline networks under various stray current interferences L. Bortels & J. Deconinck Department of Electrical Engineering (TW-ETEC), Vrije Universiteit
Corrosion inhibition of aluminum and aluminum silicon alloys in sodium hydroxide solutions by methyl cellulose Salah Eid*, M. Abdallah, E. M. Kamar, A. Y. El-Etre Chemistry department, Faculty of science,
REPRODUCIBILITY OF CRITICAL CHLORIDE THRESHOLD LEVELS FOR STAINLESS STEEL REINFORCEMENT S. Randström, M. Almén, R. Pettersson Outokumpu Stainless AB Avesta Research Centre SE-774 22 Avesta Sweden firstname.lastname@example.org